Low-Temperature Chemoselective Gold-Surface-Mediated Hydrogenation of Acetone and Propionaldehyde Ming Pan,[a] Zachary D. Pozun,[b] Adrian J. Brush,[a] Graeme Henkelman,[b] and C. Buddie Mullins*[a] Since nanoscale gold was first discovered to be catalytically active, gold-based catalysts have been studied both theoretically and experimentally in a wide range of reactions. These catalysts exhibit high activity for hydrogenation processes, in particular showing enhanced selectivity. However, there is a lack of relevant fundamental studies into these processes. Conducting hydrogenation reactions on model gold surfaces is useful for obtaining mechanistic insight and for further enhancing our understanding of the catalytic properties of supported-gold catalysts. Herein, we report the chemoselective hydrogenation of aldehydes over ketones on gold surfaces. The hydrogenation chemistry of oxygenated hydrocarbons has been studied on transition-metal surfaces for a variety of reactions that are important to the pharmaceutical- and chemical industries. For example, C=O bond hydrogenation is a key step in the catalytic conversion of cellulosic biomass. In addition, gold-based catalysts have also shown exceptional activity for the selective hydrogenation of a,b-unsaturated carbonyl compounds. Claus found that, in the production of allyl alcohol from the hydrogenation of acrolein, gold catalysts yielded about 10-times-higher selectivity for C=O bond hydrogenation than traditional platinum-based catalysts. Therefore, exploring the individual reactivity of carbonyl-hydrogenation could provide useful information for a better holistic understanding of these important catalytic reactions. By employing propionaldehyde and acetone as representative probe molecules of aldehydes and ketones, respectively, we investigated the hydrogenation of C=O bonds on a model pre-atomic-hydrogen-covered Au(111) catalyst. H atoms were used herein owing to the high energetic barrier of H2-dissociation on gold. Temperature-programmed-desorption (TPD) measurements indicated different activities for hydrogenation on gold: propionaldehyde underwent hydrogenation to afford 1-propanol on H-covered gold but acetone did not form 2propanol. Density functional theory (DFT) calculations revealed different activation energies for the reactions between a single carbonyl moiety and a H atom. [a] M. Pan, A. J. Brush, Prof. C. B. Mullins Department of Chemical Engineering University of Texas at Austin Austin, TX 78703-0231 (USA) Fax: (+ 1) 512-471-7060 E-mail: [email protected]
[b] Dr. Z. D. Pozun, Prof. G. Henkelman Department of Chemistry and Biochemistry Institute for Computational Engineering and Sciences University of Texas at Austin Austin, TX 78712-0165 (USA) Supporting information for this article is available on the WWW under http://dx.doi.org/10.1002/cctc.201200311.
ChemCatChem 2012, 4, 1241 – 1244
First, the hydrogenation of acetone was investigated on a Au(111) surface. In a control experiment (Figure 1 a), 1.62 ML (ML = monolayer) of acetone (m/z = 43, the most-abundant mass fragment of acetone) was adsorbed onto a clean Au(111)
Figure 1. TPD spectra following the adsorption of acetone (1.62 ML) on: a) clean- and b) pre-atomic-hydrogen-covered (qH,rel = 1) Au(111) surfaces. All species were adsorbed onto the surface at 77 K. The heating rate was 1 K s 1. Spectra (a) and (b) have the same scale for the y axis.
surface. Upon heating to 300 K with a ramp rate of 1 K s 1, two desorption features appeared: second-layer desorption at 132 K and monolayer desorption at 155 K. With increasing acetone coverage, multilayer desorption created a distinct feature at 126–131 K (see the Supporting Information, Figure S1). Our TPD data was in excellent agreement with the results by Syomin and Koel. The signal from m/z = 58 (parent mass of acetone) was also monitored to verify the desorption of CH3COCH3. On the pre-atomic-hydrogen-covered Au(111) surface, the thermal desorption spectrum of acetone changed significantly (Figure 1 b). Compared to the clean Au(111) surface, H atoms caused the desorption features to broaden. These interactions also shifted the monolayer desorption to a slightly higher temperature (158 K) and resulted in the appearance of two new desorption features at 195 and 210 K. However, no hydrogenated products (e.g., 2-propanol at m/z = 45) were observed. Furthermore, no deuterated 2-propanol was generated from either H+CD3COCD3 or D+CH3COCH3. These results clearly indicated that, whereas there were noticeable interactions be-
2012 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim
tween acetone and hydrogen on the Au(111) surface, the catalytic activity was not high enough to initiate a reaction. To assess gold as a hydrogenation catalyst for aldehydes as compared to ketones, we investigated the hydrogenation of propionaldehyde. Figure 2 shows TPD measurements of propionaldehyde on clean- (Figure 2 a) and pre-adsorbed-hydro-
Figure 2. TPD spectra following the adsorption of propionaldehyde (1.82 ML) on: a) clean- and b) pre-atomic-hydrogen-covered (qH,rel = 1) Au(111) surfaces. All species were adsorbed onto the surface at 77 K. The heating rate was 1 K s 1. Spectra (a) and (b) have the same scale for the y axis.
gen-covered (Figure 2 b) Au(111) surfaces. On the clean surface, 1.82 ML of propionaldehyde, which was represented by both the m/z = 29 (CH3CH2 and CHO) and m/z = 31 fragments (CH18O; from the natural abundance of 18O), yielded multilayerand monolayer-desorption features at 121 and 154 K, respectively. We also observed another desorption feature at 269 K, which was presumably associated with the polymerization of CH3CH2CHO on the clean surface. The polymerization of aldehydes has been widely reported on many metal surfaces, including Ru, Au, Cu, and Pd. For more-detailed information on the desorption of propionaldehyde with various coverages, see the Supporting Information, Figure S2. Figure 2 b shows TPD measurements following the co-adsorption of 1.82 ML of CH3CH2CHO and H atoms (qH,rel = 1) on a Au(111) surface at 77 K. With the co-adsorption of H atoms, the TPD-desorption spectra for propionaldehyde (m/z = 29) showed several changes. Although the polymerization feature remained at 271 K, its integrated area was smaller than that of propionaldehyde on a clean Au(111) surface. In addition, we observed a small desorption feature at 147 K, a strong, sharp feature at 186 K, and a small feature at 220 K. The origins of these three peaks are unclear and more studies are required to understand them from a mechanistic point of view. The spec-
tra for m/z = 31 (Figure 2 b) displayed the expected small peaks at 186 K and 271 K, which corresponded to the natural abundance of CH18O from the desorption of propionaldehyde (about 3 % of m/z = 29 as in Figure 2 a). However, the desorption peak at 220 K for the m/z = 31 curve was much larger than would be expected from natural abundance alone, thus indicating that 1-propanol was formed. We estimated that 90 % of the m/z = 31 desorption peak at about 220 K could be assigned to 1-propanol. The production of CH3CH2CH2OH was confirmed by the parent mass-fragment peak of 1-propanol, m/z = 60, with the same shape and temperature (see the Supporting Information, Figure S3). Comparison between the reactions of acetone and propionaldehyde with H atoms revealed a higher reactivity of CH3CH2CHO on Au(111) surfaces and suggested chemoselectivity for the hydrogenation reaction on the gold surface. We used DFT calculations (for methods, see the Supporting Information) to understand the mechanisms on a molecular/atomic scale, similar to the study performed by Alcala and co-workers on a model Pt(111) surface. They found that the hydrogenation of propionaldehyde was more-favorable owing to its lower activation energy (0.54 eV) than acetone (0.76 eV). They asserted that the hydrogenation of the carbonyl-carbon atom is the first step, followed by the hydrogenation of the oxygen species. However, our DFT calculations (Figure 3) suggested different reaction pathways and mechanisms on a gold surface. Acetone and propionaldehyde are structural isomers of one another. Acetone was calculated to be 0.33 eV lower in energy than propionaldehyde in the gas phase, owing to the higher thermodynamic stability of ketones compared to aldehydes. Our DFT calculations indicated that both species weakly chemisorbed onto the pre-atomic-hydrogen-covered gold surface (dispersion forces were not included in these calculations). Notably, whilst our DFT calculations indicated similar desorption energies for acetone and propionaldehyde, the TPD data for propionaldehyde (Figure 2 b) indicated a significantly higher desorption energy than acetone (Figure 1 b). This result is presumably due to the fact that these DFT calculations modeled single molecules and did not account for interactions between multiple surface species. Despite this discrepancy, our DFT calculations give valuable mechanistic insight into the chemoselectivity of gold by comparing the transition-state energies for the partially hydrogenated intermediates (see below). The key step that anchors the molecules onto the surface is the hydrogenation of the carbonyl-oxygen atom. In each case, this process had a barrier of 0.2 eV. Following hydrogenation, the carbonyl-carbon atom became sp3 hybridized and formed a covalent bond with a surface gold atom. This process is shown in Figure 3, which shows the displacement of the gold atom out of the surface owing to covalent interactions (Figure 3, panels 2 A and 2 B). Owing to the increased steric demands of the bulky methyl groups at the carbonyl-carbon positions in acetone, this protonation step was only exothermic by 0.1 eV. In contrast, hydrogenated propionaldehyde faced less steric interactions with the surface and the hydrogenation step was exothermic by over 0.4 eV.
2012 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim
ChemCatChem 2012, 4, 1241 – 1244
molecules was higher at increased temperature such that the polymer may dissociate and undergo full hydrogenation. This result was also consistent with our observation that propionaldehyde showed a concomitant desorption feature with produced 1-propanol at 220 K (Figure 2 b), which has also been observed in the hydrogenation of acetaldehyde on a Au(111) surface. In contrast, acetone did not polymerize; thus, desorption from the surface at lower temperatures remained favorable compared to hydrogenation. As shown in Figure 2 b, we also observed the desorption of di-n-propyl ether (CH3CH2CH2OCH2CH2CH3) from propionaldehyde on H-covered Au(111) surfaces. This species is represented by the curve for m/z = 73, with a desorption feature that was centered at 225 K, and was verified by two other characteristic mass fragments at m/z = 43 and 102 (see the Supporting Information, Figure S3); the fragment at m/z = 43 was the most-abundant fragment and that at 102 was the parent mass. Figure 2 a shows that the di-n-propyl ether did not originate from impurities in the reactant and strongly suggests that the compound was formed from a couFigure 3. Energy diagram for the hydrogenation of acetone and propionaldehyde on pling reaction of propionaldehyde. Water-desorption a Au(111) surface. was observed at 180 K and further supported the conclusion that the ether was formed through Following the initial hydrogenation of the carbonyl-oxygen a mechanism that was akin to the standard acid-catalyzed deatom, the carbonyl-carbon atom is vulnerable to attack by surhydration reaction in solution. A more-detailed study regarding face hydrogen atoms. Although this reaction is highly exotherthe related reaction mechanisms is underway. mic in both cases, Figure 3 shows a possible explanation for Isotope experiments were performed to further investigate the observance of 1-propanol and not 2-propanol. The barrier the reaction mechanisms. First, we studied the hydrogenation to hydrogenation of the carbonyl-carbon atom in propionaldereaction between CH3CH2CHO and D atoms (Figure 4 a), where hyde is significantly lower than the barrier to return the initial 1.86 ML of propionaldehyde was adsorbed onto a deuterated hydrogen atom to the surface. In contrast, acetone has a lower Au(111) surface (qD,rel = 1). The TPD spectrum for m/z = 33 disbarrier for returning the initial hydrogen atom to the surface played a peak at 220 K, which was the same temperature as than that for hydrogenation of the carbonyl-carbon atom. the desorption of 1-propanol in Figure 2 b, and indicated the Therefore, for the partially hydrogenated intermediates, the production of CH3CH2CHDOD, which was verified by the detecpropionaldehyde intermediate is most likely to proceed to the tion of the corresponding parent mass (62, not shown). In adfully hydrogenated 1-propanol, whereas the acetone interdition, we detected partially deuterated di-n-propyl ether mediate is most likely to reverse back to give the adsorbed (CH3CH2CHDOCHDCH2CH3) with a characteristic mass fragment acetone. at m/z = 75 and a desorption peak at 225 K. Desorption peaks An additional- and possibly more-important factor that of the mass fragment m/z = 44 and of the parent mass (m/z = favors the hydrogenation of propionaldehyde is the polymeri104) were also observed (not shown). zation reaction. Comparison of Figure 1 a and Figure 2 a shows In addition, these isotopic experiments provided insight into that propionaldehyde polymerizes on the clean surface, as inthe kinetic isotope effect (KIE) on the surface reactions. Figdicated by the desorption peak at 269 K, but acetone does ure 4 b shows the integrated areas under the desorption feanot. A similar phenomenon also occurred on the H-covered tures of products 1-propanol (m/z = 31 and 33) and di-n-propyl Au(111) surface. Hydrogenation of the carbonyl-oxygen atom ether (m/z = 73 and 75) as an indicator of their corresponding activated the carbonyl-carbon atom, thereby allowing strong production in the H- and D-reaction systems. These results ininteractions with the oxygen atom of another molecule. As dicated a lower reactivity of deuterium for the surface reacshown in the Supporting Information, Figure S4, polymeritions and showed values of 2.9 for the ratio of m/z = 31 to m/ zation with a second surface molecule was exothermic by z = 33 (thus indicating the production of 1-propanol) and 1.3 0.45 eV in propionaldehyde and endothermic by 0.3 eV in acefor the ratio of m/z = 73 to m/z = 75 (thus indicating the protone. Thus, these polymerization reactions help to account for duction of the ether). Thus, we concluded that the reaction bethe increased susceptibility of propionaldehyde towards hydrotween propionaldehyde and H atoms was influenced by a KIE, genation. The more-strongly bound polymer desorbed at which was comparably stronger for the hydrogenation of proa much-higher temperature, so the concentration of surface pionaldehyde than for the formation of di-n-propyl ether. ChemCatChem 2012, 4, 1241 – 1244
2012 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim
Acknowledgements We thank the Department of Energy (DE-FG02-04ER15587) and the Welch Foundation (F-1436 for C.B.M., F-1601 for G.H.) for their support. M.P. acknowledges the William S. Livingston Fellowship, and Z.D.P. acknowledges the Dorothy B. Banks Fellowship for financial support. Keywords: acetone · chemoselectivity · gold · hydrogenation · propionaldehyde
Figure 4. a) TPD spectra following the adsorption of propionaldehyde (1.82 ML) onto a pre-atomic-deuterium-covered (qD,rel = 1) Au(111) surface. b) Production of 1-propanol and di-n-propyl ether from the H- and D-covered surface. All species were adsorbed onto the surface at 77 K. The heating rate was 1 K s 1.
In summary, acetone formed weak interactions with atomic H atoms on a Au(111) surface, as indicated by the TPD-desorption spectra. However, no hydrogenated product was observed. In contrast, the hydrogenation of propionaldehyde was detected by the production of 1-propanol. DFT calculations predicted similar energetic barriers for the initial hydrogenation reaction; however, the reverse reaction for acetone was favored over the final hydrogenation step. Conversely, the full hydrogenation reaction for propionaldehyde was favored over the reverse reaction. In addition, the polymerization of CH3CH2CHO on a Au(111) surface was exothermic and may play a role in the hydrogenation reaction by increasing the surface concentration of propionaldehyde. Di-n-propyl ether can be generated by a coupling reaction of propionaldehyde on Hcovered Au(111) and is likely generated in the reaction between surface intermediates and the produced alcohol. Deuterium-labeling experiments showed lowered reactivity for the production of both 1-propanol and di-n-propyl ether, thereby indicating the presence of a kinetic isotope effect.
Experimental Section All of the experiments were performed in an ultrahigh-vacuum (UHV) supersonic-molecular-beam apparatus with a base pressure of 2 10 10 Torr. A quadrupole mass spectrometer (QMS) was used to monitor the gas-phase species that desorbed from the sample surface. H atoms were generated with a homemade electron-beam-heated device. For details of the experimental procedure, see the Supporting Information.
 a) G. C. Bond, P. A. Sermon, G. Webb, D. A. Buchanan, P. B. Wells, J. Chem. Soc. Chem. Commun. 1973, 444 – 445; b) W. S. Epling, G. B. Hoflund, J. F. Weaver, S. Tsubota, M. Haruta, J. Phys. Chem. 1996, 100, 9929 – 9934; c) M. Haruta, Catal. Today 1997, 36, 153 – 166.  a) T. A. Baker, X. Y. Liu, C. M. Friend, Phys. Chem. Chem. Phys. 2011, 13, 34 – 46; b) J. Greeley, M. Mavrikakis, J. Phys. Chem. B 2005, 109, 3460 – 3471.  a) J. L. Gong, C. B. Mullins, J. Am. Chem. Soc. 2008, 130, 16458 – 16459; b) J. L. Gong, C. B. Mullins, Acc. Chem. Res. 2009, 42, 1063 – 1073; c) J. Kim, Z. Dohnlek, B. D. Kay, J. Am. Chem. Soc. 2005, 127, 14592 – 14593; d) B. K. Min, C. M. Friend, Chem. Rev. 2007, 107, 2709 – 2724; e) S. D. Senanayake, D. Stacchiola, P. Liu, C. B. Mullins, J. Hrbek, J. A. Rodriguez, J. Phys. Chem. C 2009, 113, 19536 – 19544.  a) J. Huang, T. Akita, J. Faye, T. Fujitani, T. Takei, M. Haruta, Angew. Chem. 2009, 121, 8002 – 8006; Angew. Chem. Int. Ed. 2009, 48, 7862 – 7866; b) R. Si, M. Flytzani-Stephanopoulos, Angew. Chem. 2008, 120, 2926 – 2929; Angew. Chem. Int. Ed. 2008, 47, 2884 – 2887.  a) J. E. Bailie, H. A. Abdullah, J. A. Anderson, C. H. Rochester, N. V. Richardson, N. Hodge, J. G. Zhang, A. Burrows, C. J. Kiely, G. J. Hutchings, Phys. Chem. Chem. Phys. 2001, 3, 4113 – 4121; b) C. Milone, M. L. Tropeano, G. Gulino, G. Neri, R. Ingoglia, S. Galvagno, Chem. Commun. 2002, 868 – 869; c) S. A. Nikolaev, V. V. Smirnov, Gold Bull. 2009, 42, 182 – 189; d) H. Sakurai, S. Tsubota, M. Haruta, Appl. Catal. A 1993, 102, 125 – 136.  a) B. Campo, M. Volpe, S. Ivanova, R. Touroude, J. Catal. 2006, 242, 162 – 171; b) T. V. Choudhary, C. Sivadinarayana, A. K. Datye, D. Kumar, D. W. Goodman, Catal. Lett. 2003, 86, 1 – 8; c) A. Corma, P. Serna, Science 2006, 313, 332 – 334; d) A. Corma, P. Serna, H. Garcia, J. Am. Chem. Soc. 2007, 129, 6358 – 6359.  a) B. Campo, C. Petit, M. A. Volpe, J. Catal. 2008, 254, 71 – 78; b) L. He, J. Ni, L. C. Wang, F. J. Yu, Y. Cao, H. Y. He, K. N. Fan, Chem. Eur. J. 2009, 15, 11833 – 11836.  R. Zheng, M. P. Humbert, Y. Zhu, J. G. Chen, Catal. Sci. Technol. 2011, 1, 638 – 643.  C. Mohr, H. Hofmeister, J. Radnik, P. Claus, J. Am. Chem. Soc. 2003, 125, 1905 – 1911.  P. Claus, Appl. Catal. A 2005, 291, 222 – 229.  B. Hammer, J. K. Norskov, Nature 1995, 376, 238 – 240.  D. Syomin, B. E. Koel, Surf. Sci. 2002, 498, 53 – 60.  M. A. Henderson, Y. Zhou, J. M. White, J. Am. Chem. Soc. 1989, 111, 1185 – 1193.  M. Pan, D. W. Flaherty, C. B. Mullins, J. Phys. Chem. Lett. 2011, 2, 1363 – 1367.  T. R. Bryden, S. J. Garrett, J. Phys. Chem. B 1999, 103, 10481 – 10488.  J. L. Davis, M. A. Barteau, J. Am. Chem. Soc. 1989, 111, 1782 – 1792.  R. Alcala, J. Greeley, M. Mavrikakis, J. A. Dumesic, J. Chem. Phys. 2002, 116, 8973 – 8980.  a) J. E. Davis, S. G. Karseboom, P. D. Nolan, C. B. Mullins, J. Chem. Phys. 1996, 105, 8362 – 8375; b) J. E. Davis, P. D. Nolan, S. G. Karseboom, C. B. Mullins, J. Chem. Phys. 1997, 107, 943 – 952; c) M. Pan, S. Hoang, J. Gong, C. B. Mullins, Chem. Commun. 2009, 7300 – 7302; d) M. Pan, S. Hoang, C. B. Mullins, Catal. Today 2011, 160, 198 – 203. Received: May 12, 2012 Published online on July 17, 2012
2012 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim
ChemCatChem 2012, 4, 1241 – 1244